text: ScBC (x = 0.27, y = 1.1, z = 0.2) has an orthorhombic crystal structure with space group Pbam (No. 55) and lattice constants of a = 1.73040(6), b = 1.60738(6) and c = 1.44829(6) nm. This phase is indicated as ScBC (phase IV) in the phase diagram of figure 17. This rare orthorhombic structure has 78 atomic positions in the unit cell: seven partially occupied Sc sites, four C sites, 66 B sites including three partially occupied sites and one B/C mixed-occupancy site. Atomic coordinates, site occupancies and isotropic displacement factors are listed in table IX.
  More than 500 atoms are available in the unit cell. In the crystal structure, there are six structurally independent icosahedra I1–I6, which are constructed from B1–B12, B13–B24, B25–B32, B33–B40, B41–B44 and B45–B56 sites, respectively; B57–B62 sites form a B polyhedron. The ScBC crystal structure is layered, as shown in figure 26. This structure has been described in terms of two kinds of boron icosahedron layers, L1 and L2. L1 consists of the icosahedra I3, I4 and I5 and the C65 "dimer", and L2 consists of the icosahedra I2 and I6. I1 is sandwiched by L1 and L2 and the B polyhedron is sandwiched by L2.
  An alternative description is based on the same B(B)supericosahedron as in the YB structure. In the YB crystal structure, the　supericosahedra form 3-dimensional boron framework as shown in figure 5. In this framework, the neighboring supericosahedra are rotated 90° with respect to each other. On the contrary, in ScBC the supericosahedra form a 2-dimensional network where the 90° rotation relation is broken because of the orthorhombic symmetry. The planar projections of the supericosahedron connection in ScBC and YB are shown in figures 27a and b, respectively. In the YB crystal structure, the neighboring 2-dimensional supericosahedron connections are out-of-phase for the rotational relation of the supericosahedron. This allows 3-dimensional
  stacking of the 2-dimensional supericosahedron connection while maintaining the cubic symmetry.
  The B boron cluster occupies the large space between four supericosahedra as described in the REB section. On the other hand, the 2-dimensional supericosahedron networks in the ScBC crystal structure stack in-phase along the z-axis. Instead of the B cluster, a pair of the I2 icosahedra fills the open space staying within the supericosahedron network, as shown in figure 28 where the icosahedron I2 is colored in yellow.
  All Sc atoms except for Sc3 reside in large spaces between the supericosahedron networks, and the Sc3 atom occupies a void in the network as shown in figure 26. Because of the small size of Sc atom, the occupancies of the Sc1–Sc5 sites exceed 95%, and those of Sc6 and Sc7 sites are approximately 90% and 61%, respectively (see table IX).